#------------------------------------------------------------------------------
#$Date: 2018-07-28 11:29:34 +0300 (Sat, 28 Jul 2018) $
#$Revision: 209293 $
#$URL: file:///home/coder/svn-repositories/cod/cif/6/00/03/6000392.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_6000392
loop_
_publ_author_name
'Lissner, Falk'
'Schleid, Thomas'
_publ_section_title
;
 Two novel sulfide chlorides of the lanthanides: Synthesis and crystal
 structure of Pr7S6Cl9 and Nd7S6Cl9
;
_journal_coden_ASTM              ZAACAB
_journal_name_full
;
 Zeitschrift Für Anorganische Und Allgemeine Chemie
;
_journal_page_first              1903
_journal_page_last               1908
_journal_paper_doi
10.1002/(SICI)1521-3749(1998110)624:11<1903::AID-ZAAC1903>3.0.CO;2-G
_journal_volume                  624
_journal_year                    1998
_chemical_formula_sum            'Cl9 Nd7 S6'
_space_group_crystal_system      monoclinic
_space_group_IT_number           13
_space_group_name_Hall           '-P 2yc'
_space_group_name_H-M_alt        'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 97.43(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   24.250(9)
_cell_length_b                   6.642(2)
_cell_length_c                   6.918(2)
_cell_volume                     1104.92
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Siemens-Stoe AED2'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_limit_h_max       1
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_theta_max         28
_diffrn_reflns_theta_min         1
_exptl_crystal_F_000             1338
_refine_ls_R_factor_all          0.060
_refine_ls_R_I_factor            0.061
_refine_ls_weighting_details     'w = 1.185σ(Fₒ)⁻²'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.048
_reflns_number_gt                2478
_reflns_number_total             2663
_reflns_threshold_expression     '|Fₒ| > 2σ(Fₒ)'
_cod_depositor_comments
;
 Adding the atomic coordinates, anisotropic parameter values, R factor values
 and additional information after consulting the original publication.

 Antanas Vaitkus,
 2018-07-29
;
_cod_database_code               6000392
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y,-z+1/2
3 -x,-y,-z
4 x,-y,z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
Nd1 Nd 2 e 0 0.2801(2) 0.25
Nd2 Nd 4 g 0.42946(3) 0.2934(1) 0.0079(1)
Nd3 Nd 4 g 0.14664(3) 0.2992(1) 0.8771(1)
Nd4 Nd 4 g 0.28849(3) 0.2981(1) 0.3636(1)
S1 S 4 g 0.3589(1) 0.5566(5) 0.1871(5)
S2 S 4 g 0.2159(1) 0.5519(5) 0.1185(5)
S3 S 4 g 0.0723(1) 0.5353(5) 0.0755(5)
Cl1 Cl 2 f 0.5 0.5591(7) 0.25
Cl2 Cl 4 g 0.3162(2) 0.0859(6) 0.0299(6)
Cl3 Cl 4 g 0.1865(2) 0.0715(6) 0.2323(5)
Cl4 Cl 4 g 0.0578(2) 0.0499(6) 0.9405(6)
Cl5 Cl 4 g 0.5607(2) 0.1009(7) 0.1247(6)
